Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Transcript

MECHANICS OF SOLIDS UNIT-I INTRODUCTION The solid mechanics as a subject may be defined as a branch of applied mechanics that deals with behaviors of solid bodies subjected to various types of loadings. This is usually subdivided into further two streams i.e Mechanics of rigid bodies or simply Mechanics and Mechanics of deformable solids.The mechanics of deformable solids which is branch of applied mechanics is known by several names i.e. strength of materials, mechanics of materials or Mechanics of solids etc. Mechanics of rigid bodies: The mechanics of rigid bodies is primarily concerned with the static and dynamic behaviour under external forces of engineering components and systems which are treated as infinitely strong and undeformable Mechanics of solids: The mechanics of deformable solids is more concerned with the internal forces and associated changes in the geometry of the components involved. Of particular importance are the properties of the materials used, the strength of which will determine whether the components fail by breaking in service, and the stiffness of which will determine whether the amount of deformation they suffer is acceptable. Therefore, the subject of mechanics of materials or strength of materials is central to the whole activity of engineering design. Usually the objectives in analysis here will be the determination of the stresses, strains, and deflections produced by loads. Theoretical analyses and experimental results have equal roles in this field. Simple stress and strain Let us introduce the concept of stress as we know that the main problem of engineering mechanics of material is the investigation of the internal resistance of the body, i.e. the nature of forces set up within a body to balance the effect of the externally applied forces. As we know that in mechanics of deformable solids, externally applied forces acts on a body and body suffers a deformation. From equilibrium point of view, this action should be opposed or reacted by internal forces which are set up within the particles of material due to cohesion. These internal forces give rise to a concept of stress. Therefore, let us define a stress Therefore, let us define a term stress Stress: Let us consider a rectangular bar of some cross – sectional area and subjected to some load or force (in Newtons ) Let us imagine that the same rectangular bar is assumed to be cut into two halves at section XX. The each portion of this rectangular bar is in equilibrium under the action of load P and the internal forces acting at the section XX has been shown Now stress is defined as the force intensity or force per unit area. Here we use a symbol σ to represent the stress. Where P is axial load and A is the cross sectional area The basic units of stress in S.I units i.e. (International system) are N / m2 (or Pa) MPa = 106 Pa GPa = 109 Pa KPa = 103 Pa Some times N / mm2 units are also used, because this is an equivalent to MPa. While US customary unit is pound per square inch psi. TYPES OF STRESSES : only two basic stresses exists : (1) normal stress and (2) shear shear stress. Other stresses either are similar to these basic stresses or are a combination of these e.g. bending stress is a combination tensile, compressive and shear stresses. Torsional stress, as encountered in twisting of a shaft is a shearing stress. Let us define the normal stresses and shear stresses in the following sections. Normal stresses : We have defined stress as force per unit area. If the stresses are normal to the areas concerned, then these are termed as normal stresses. The normal stresses are generally denoted by a Greek letter ( σ ) This is also known as uniaxial state of stress, because the stresses acts only in one direction however, such a state rarely exists, therefore we have biaxial and triaxial state of stresses where either the two mutually perpendicular normal stresses acts or three mutually perpendicular normal stresses acts as shown in the figures below : Tensile or compressive stresses : The normal stresses can be either tensile or compressive whether the stresses acts out of the area or into the area Shear stresses : Let us consider now the situation, where the cross – sectional area of a block of material is subject to a distribution of forces which are parallel, rather than normal, to the area concerned. Such forces are associated with a shearing of the material, and are referred to as shear forces. The resulting force intensities are known as shear stresses, the mean shear stress being equal to Where P is the total force and A the area over which it acts. The greek symbol τ ( tau ) ( suggesting tangential ) is used to denote shear stress. . STRESS - STRAIN RELATIONS Stress – Strain Relations: The Hook's law, states that within the elastic limits the stress is proportional to the strain since for most materials it is impossible to describe the entire stress – strain curve with simple mathematical expression, in any given problem the behavior of the materials is represented by an idealized stress – strain curve, which emphasizes those aspects of the behaviors which are most important is that particular problem. Elastic Stress – strain Relations : Previously stress – strain relations were considered for the special case of a uniaxial loading i.e. only one component of stress i.e. the axial or normal component of stress was coming into picture. In this section we shall generalize the elastic behavior, so as to arrive at the relations which connect all the six components of stress with the six components of elastic stress. Futher, we would restrict overselves to linearly elastic material. ISOTROPIC: If the response of the material is independent of the orientation of the load axis of the sample, then we say that the material is isotropic or in other words we can say that isotropy of a material in a characteristics, which gives us the information that the properties are the same in the three orthogonal directions x y z, on the other hand if the response is dependent on orientation it is known as anisotropic. Examples of anisotropic materials, whose properties are different in different directions are (i) Wood (ii) Fibre reinforced plastic (iii) Reinforced concrete HOMOGENIUS: A material is homogenous if it has the same composition through our body. Hence the elastic properties are the same at every point in the body. However, the properties need not to be the same in all the direction for the material to be homogenous. Isotropic materials have the same elastic properties in all the directions. Therefore, the material must be both homogenous and isotropic in order to have the lateral strains to be same at every point in a particular component. Poissons Ratio: the ratio of lateral strain to longitudinal strain These equation expresses the relationship between stress and strain (Hook's law) for uniaxial state of stress only when the stress is not greater than the proportional limit. In order to analyze the deformational effects produced by all the stresses, we shall consider the effects of one axial stress at a time. Since we presumably are dealing with strains of the order of one percent or less. These effects can be superimposed arbitrarily. The figure below shows the general triaxial state of stress. Let us consider a case when σx alone is acting. It will cause an increase in dimension in Xdirection whereas the dimensions in y and z direction will be decreased. Therefore the resulting strains in three directions are Similarly let us consider that normal stress σy alone is acting and the resulting strains are Now let us consider the stress σz acting alone, thus the strains produced are ELASTIC CONSTANTS In considering the elastic behavior of an isotropic materials under, normal, shear and hydrostatic loading, we introduce a total of four elastic constants namely E, G, K, and . It turns out that not all of these are independent to the others. In fact, given any two of them, the other two can be foundout . Let us define these elastic constants (i) E = Young's Modulus of Rigidity = Stress / strain (ii) G = Shear Modulus or Modulus of rigidity = Shear stress / Shear strain (iii) = Possion's ratio = lateral strain / longitudinal strain (iv) K = Bulk Modulus of elasticity = Volumetric stress / Volumetric strain Where Volumetric strain = sum of linear stress in x, y and z direction. Volumetric stress = stress which cause the change in volume. Let us find the relations between them Relation between E, G and : Let us establish a relation among the elastic constants E,G and . Consider a cube of material of side „a' subjected to the action of the shear and complementary shear stresses as shown in the figure and producing the strained shape as shown in the figure below. Assuming that the strains are small and the angle A C B may be taken as 450. Therefore strain on the diagonal OA = Change in length / original length Since angle between OA and OB is very small hence OA & OB therefore BC, is the change in the length of the diagonal OA Now this shear stress system is equivalent or can be replaced by a system of direct stresses at 450 as shown below. One set will be compressive, the other tensile, and both will be equal in value to the applied shear strain. Thus, for the direct state of stress system which applies along the diagonals: We have introduced a total of four elastic constants, i.e E, G, K and μ. It turns out that not all of these are independent of the others. Infact given any two of then, the other two can be found. irrespective of the stresses i.e, the material is incompressible. When μ= 0.5 Value of k is infinite, rather than a zero value of E and volumetric strain is zero, or in other words, the material is incompressible. Relation between E, K and : Consider a cube subjected to three equal stresses as shown in the figure below The total strain in one direction or along one edge due to the application of hydrostatic stress or volumetric stress is given as Relation between E, G and K : The relationship between E, G and K can be easily determained by eliminating from the already derived relations E = 2 G ( 1 + μ ) and E = 3 K ( 1-2μ) Thus, the following relationship may be obtained Relation between E, K and : From the already derived relations, E can be eliminated Engineering Brief about the elastic constants : We have introduced a total of four elastic constants i.e E, G, K and . It may be seen that not all of these are independent of the others. Infact given any two of them, the other two can be determined. Futher, it may be noted that hence if = 0.5, the value of K becomes infinite, rather than a zero value of E and the volumetric strain is zero or in otherwords, the material becomes incompressible Futher, it may be noted that under condition of simple tension and simple shear, all real materials tend to experience displacements in the directions of the applied forces and Under hydrostatic loading they tend to increase in volume. In otherwords the value of the elastic constants E, G and K cannot be negative Therefore, the relations E=2G(1+μ) E = 3 K ( 1 -2μ ) Yields In actual practice no real material has value of Poisson's ratio negative . Thus, the value of cannot be greater than 0.5, if however 0.5 than v = ve, which is physically unlikely because when the material is stretched its volume would always increase. Determination of Poisson's ratio: Poisson's ratio can be determined easily by simultaneous use of two strain gauges on a test specimen subjected to uniaxial tensile or compressive load. One gage is mounted parallel to the longitudnal axis of the specimen and other is mounted perpendicular to the longitudnal axis as shown below: MECHANICAL PROPERTIES Mechanical Properties: In the course of operation or use, all the articles and structures are subjected to the action of external forces, which create stresses that inevitably cause deformation. To keep these stresses, and, consequently deformation within permissible limits it is necessary to select suitable materials for the Components of various designs and to apply the most effective heat treatment. i.e. a Comprehensive knowledge of the chief character tics of the semi-finished metal products & finished metal articles (such as strength, ductility, toughness etc) are essential for the purpose. For this reason the specification of metals, used in the manufacture of various products and structure, are based on the results of mechanical tests or we say that the mechanical tests conducted on the specially prepared specimens (test pieces) of standard form and size on special machines to obtained the strength, ductility and toughness characteristics of the metal. The conditions under which the mechanical test are conducted are of three types (1) Static: When the load is increased slowly and gradually and the metal is loaded by tension, compression, torsion or bending. (2) Dynamic: when the load increases rapidly as in impact (3) Repeated or Fatigue: (both static and impact type) . i.e. when the load repeatedly varies in the course of test either in value or both in value and direction Now let us consider the uniaxial tension test. [ For application where a force comes on and off the structure a number of times, the material cannot withstand the ultimate stress of a static tool. In such cases the ultimate strength depends on no. of times the force is applied as the material works at a particular stress level. Experiments one conducted to compute the number of cycles requires to break to specimen at a particular stress when fatigue or fluctuating load is acting. Such tests are known as fatque tests ] Uniaxial Tension Test: This test is of static type i.e. the load is increased comparatively slowly from zero to a certain value. Standard specimen's are used for the tension test. There are two types of standard specimen's which are generally used for this purpose, which have been shown below: Specimen I: This specimen utilizes a circular X-section. Specimen II: This specimen utilizes a rectangular X-section. lg = gauge length i.e. length of the specimen on which we want to determine the mechanical properties.The uniaxial tension test is carried out on tensile testing machine and the following steps are performed to conduct this test. (i) The ends of the specimen's are secured in the grips of the testing machine. (ii) There is a unit for applying a load to the specimen with a hydraulic or mechanical drive. (iii) There must be a some recording device by which you should be able to measure the final output in the form of Load or stress. So the testing machines are often equipped with the pendulum type lever, pressure gauge and hydraulic capsule and the stress Vs strain diagram is plotted which has the following shape. A typical tensile test curve for the mild steel has been shown below Nominal stress – Strain OR Conventional Stress – Strain diagrams: Stresses are usually computed on the basis of the original area of the specimen; such stresses are often referred to as conventional or nominal stresses. True stress – Strain Diagram: Since when a material is subjected to a uniaxial load, some contraction or expansion always takes place. Thus, dividing the applied force by the corresponding actual area of the specimen at the same instant gives the so called true stress. SALIENT POINTS OF THE GRAPH: (A) So it is evident form the graph that the strain is proportional to strain or elongation is proportional to the load giving a st.line relationship. This law of proportionality is valid upto a point A. or we can say that point A is some ultimate point when the linear nature of the graph ceases or there is a deviation from the linear nature. This point is known as the limit of proportionality or the proportionality limit. (B) For a short period beyond the point A, the material may still be elastic in the sense that the deformations are completely recovered when the load is removed. The limiting point B is termed as Elastic Limit . (C) and (D) - Beyond the elastic limit plastic deformation occurs and strains are not totally recoverable. There will be thus permanent deformation or permanent set when load is removed. These two points are termed as upper and lower yield points respectively. The stress at the yield point is called the yield strength. A study a stress – strain diagrams shows that the yield point is so near the proportional limit that for most purpose the two may be taken as one. However, it is much easier to locate the former. For material which do not posses a well define yield points, In order to find the yield point or yield strength, an offset method is applied. In this method a line is drawn parallel to the straight line portion of initial stress diagram by off setting this by an amount equal to 0.2% of the strain as shown as below and this happens especially for the low carbon steel. (E) A further increase in the load will cause marked deformation in the whole volume of the metal. The maximum load which the specimen can with stand without failure is called the load at the ultimate strength. The highest point „E' of the diagram corresponds to the ultimate strength of a material. σu = Stress which the specimen can with stand without failure & is known as Ultimate Strength or Tensile Strength. σu is equal to load at E divided by the original cross-sectional area of the bar. (F) Beyond point E, the bar begins to forms neck. The load falling from the maximum until fracture occurs at F. [ Beyond point E, the cross-sectional area of the specimen begins to reduce rapidly over a relatively small length of bar and the bar is said to form a neck. This necking takes place whilst the load reduces, and fracture of the bar finally occurs at point F ] Note: Owing to large reduction in area produced by the necking process the actual stress at fracture is often greater than the above value. Since the designers are interested in maximum loads which can be carried by the complete cross section, hence the stress at fracture is seldom of any practical value. Percentage Elongation: 'δ': The ductility of a material in tension can be characterized by its elongation and by the reduction in area at the cross section where fracture occurs. It is the ratio of the extension in length of the specimen after fracture to its initial gauge length, expressed in percent. lI = gauge length of specimen after fracture(or the distance between the gage marks at fracture) lg= gauge length before fracture(i.e. initial gauge length) For 50 mm gage length, steel may here a % elongation of the order of 10% to 40%. Elastic Action: The elastic is an adjective meaning capable of recovering size and shape after deformation. Elastic range is the range of stress below the elastic limit. Many engineering materials behave as indicated in Fig(a) however, some behaves as shown in figures in (b) and (c) while in elastic range. When a material behaves as in (c), the vsis not single valued since the strain corresponding to any particular „ ' will depend upon loading history. Fig (d): It illustrates the idea of elastic and plastic strain. If a material is stressed to level (1) and then relased the strain will return to zero beyond this plastic deformation remains. If a material is stressed to level (2) and then released, the material will recover the amount (2 2p ), where 2p is the plastic strain remaining after the load is removed. Similarly for level (3) the plastic strain will be3p. Ductile and Brittle Materials: Based on this behaviour, the materials may be classified as ductile or brittle materials Ductile Materials: It we just examine the earlier tension curve one can notice that the extension of the materials over the plastic range is considerably in excess of that associated with elastic loading. The Capacity of materials to allow these large deformations or large extensions without failure is termed as ductility. The materials with high ductility are termed as ductile materials. Brittle Materials: A brittle material is one which exhibits a relatively small extensions or deformations to fracture, so that the partially plastic region of the tensile test graph is much reduced. This type of graph is shown by the cast iron or steels with high carbon contents or concrete. Conditions Affecting Mechanical Properties: The Mechanical properties depend on the test conditions (1) It has been established that lowering the temperature or increasing the rate of deformation considerably increases the resistance to plastic deformation. Thus, at low temperature (or higher rates of deformation), metals and alloys, which are ductile at normal room temperature may fail with brittle fracture. (2) Notches i.e. sharp charges in cross sections have a great effect on the mechanical properties of the metals. A Notch will cause a non – uniform distribution of stresses. They will always contribute lowering the ductility of the materials. A notch reduces the ultimate strength of the high strength materials. Because of the non – uniform distribution of the stress or due to stress concentration. (3) Grain Size : The grain size also affects the mechanical properties. Hardness: Hardness is the resistance of a metal to the penetration of another harder body which does not receive a permanent set. Hardness Tests consists in measuring the resistance to plastic deformation of layers of metals near the surface of the specimen i.e. there are Ball indentation Tests. Ball indentation Tests: iThis method consists in pressing a hardened steel ball under a constant load P into a specially prepared flat surface on the test specimen as indicated in the figures below : After removing the load an indentation remains on the surface of the test specimen. If area of the spherical surface in the indentation is denoted as F sq. mm. Brinell Hardness number is defined as : Bhn = P / F F is expressed in terms of D and d D = ball diameter d = diametric of indentation and Brinell Hardness number is given by Then is there is also Vicker's Hardness Number in which the ball is of conical shape. IMPACT STRENGTH Static tension tests of the unnotched specimen's do not always reveal the susceptibility of metal to brittle fracture. This important factor is determined in impact tests. In impact tests we use the notched specimen's this specimen is placed on its supports on anvil so that blow of the striker is opposite to the notch the impact strength is defined as the energy A, required to rupture the specimen, Impact Strength = A / f Where f = It is the cross – section area of the specimen in cm2 at fracture & obviously at notch. The impact strength is a complex characteristic which takes into account both toughness and strength of a material. The main purpose of notched – bar tests is to study the simultaneous effect of stress concentration and high velocity load application Impact test are of the severest type and facilitate brittle friction. Impact strength values can not be as yet be used for design calculations but these tests as rule provided for in specifications for carbon & alloy steels.Futher, it may be noted that in impact tests fracture may be either brittle or ductile. In the case of brittle fracture, fracture occurs by separation and is not accompanied by noticeable plastic deformation as occurs in the case of ductile fracture. Members Subjected to Uniaxial Stress Members in Uni – axial state of stress Introduction: [For members subjected to uniaxial state of stress] For a prismatic bar loaded in tension by an axial force P, the elongation of the bar can be determined as Suppose the bar is loaded at one or more intermediate positions, then equation (1) can be readily adapted to handle this situation, i.e. we can determine the axial force in each part of the bar i.e. parts AB, BC, CD, and calculate the elongation or shortening of each part separately, finally, these changes in lengths can be added algebraically to obtain the total charge in length of the entire bar. When either the axial force or the cross – sectional area varies continuosly along the axis of the bar, then equation (1) is no longer suitable. Instead, the elongation can be found by considering a deferential element of a bar and then the equation (1) becomes i.e. the axial force Pxand area of the cross – section Ax must be expressed as functions of x. If the expressions for Pxand Ax are not too complicated, the integral can be evaluated analytically, otherwise Numerical methods or techniques can be used to evaluate these integrals. stresses in Non – Uniform bars Consider a bar of varying cross section subjected to a tensile force P as shown below. Let a = cross sectional area of the bar at a chosen section XX then Stress = p / a If E = Young's modulus of bar then the strain at the section XX can be calculated = / E Then the extension of the short element x. =.original length = / E. x Now let us for example take a case when the bar tapers uniformly from d at x = 0 to D at x = l In order to compute the value of diameter of a bar at a chosen location let us determine the value of dimension k, from similar triangles therefore, the diameter 'y' at the X-section is or = d + 2k Hence the cross –section area at section X- X will be hence the total extension of the bar will be given by expression An interesting problem is to determine the shape of a bar which would have a uniform stress in it under the action of its own weight and a load P. let us consider such a bar as shown in the figure below: The weight of the bar being supported under section XX is The same results are obtained if the bar is turned upside down and loaded as a column as shown in the figure below: IIIustrative Problem 1: Calculate the overall change in length of the tapered rod as shown in figure below. It carries a tensile load of 10kN at the free end and at the step change in section a compressive load of 2 MN/m evenly distributed around a circle of 30 mm diameter take the value of E = 208 GN / m2. This problem may be solved using the procedure as discussed earlier in this section IIIustrative Problem 2: A round bar, of length L, tapers uniformly from radius r1 at one end to radius r2at the other. Show that the extension produced by a tensile axial load P is If r2 = 2r1 , compare this extension with that of a uniform cylindrical bar having a radius equal to the mean radius of the tapered bar. Solution: consider the above figure let r1 be the radius at the smaller end. Then at a X crosssection XX located at a distance x from the smaller end, the value of radius is equal to Comparing of extensions For the case when r2 = 2.r1, the value of computed extension as above becomes equal to The mean radius of taper bar = 1 / 2( r1 + r2 ) = 1 / 2( r1 +2 r2 ) = 3 / 2 .r1 Therefore, the extension of uniform bar = Orginal length . strain Thermal stresses, Bars subjected to tension and Compression Compound bar: In certain application it is necessary to use a combination of elements or bars made from different materials, each material performing a different function. In over head electric cables or Transmission Lines for example it is often convenient to carry the current in a set of copper wires surrounding steel wires. The later being designed to support the weight of the cable over large spans. Such a combination of materials is generally termed compound bars. Consider therefore, a compound bar consisting of n members, each having a different length and cross sectional area and each being of a different material. Let all member have a common extension „x' i.e. the load is positioned to produce the same extension in each member. Where Fn is the force in the nth member and An and Ln are its cross - sectional area and length. Let W be the total load, the total load carried will be the sum of all loads for all the members. Therefore, each member carries a portion of the total load W proportional of EA / L value. The above expression may be writen as if the length of each individual member in same then, we may write Thus, the stress in member '1' may be determined as 1 = F1 / A1 Determination of common extension of compound bars: In order to determine the common extension of a compound bar it is convenient to consider it as a single bar of an imaginary material with an equivalent or combined modulus Ec. Assumption: Here it is necessary to assume that both the extension and original lengths of the individual members of the compound bar are the same, the strains in all members will than be equal. Total load on compound bar = F1 + F2+ F3 +………+ Fn where F1 , F 2 ,….,etc are the loads in members 1,2 etc But force = stress . area,therefore (A 1 + A 2 + ……+ A n ) = 1 A1 + 2 A2 + ........+n An Where is the stress in the equivalent single bar Dividing throughout by the common strain. Compound bars subjected to Temp. Change : Ordinary materials expand when heated and contract when cooled, hence , an increase in temperature produce a positive thermal strain. Thermal strains usually are reversible in a sense that the member returns to its original shape when the temperature return to its original value. However, there here are some materials which do not behave in this manner. These metals differs from ordinary materials in a sence that the strains are related non linearly to temperature and some times are irreversible .when a material is subjected to a change in temp. is a length will change by an amount. t = .L.t ort.L.t or t= E ..t = coefficient of linear expansoin for the material L = original Length t = temp. change Thus an increase in temperature produces an increase in length and a decrease in temperature results in a decrease in length except in very special cases of materials with zero or negative coefficients of expansion which need not to be considered here. If however, the free expansion of the material is prevented by some external force, then a stress is set up in the material. They stress is equal in magnitude to that which would be produced in the bar by initially allowing the bar to its free length and then applying sufficient force to return the bar to its original length. Change in Length = L t Therefore, strain = L t / L = t Therefore ,the stress generated in the material by the application of sufficient force to remove this strain = strain x E or Stress = E t Consider now a compound bar constructed from two different materials rigidly joined together, for simplicity. Let us consider that the materials in this case are steel and brass. If we have both applied stresses and a temp. change, thermal strains may be added to those given by generalized hook's law equation –e.g. While the normal strains a body are affected by changes in temperatures, shear strains are not. Because if the temp. of any block or element changes, then its size changes not its shape therefore shear strains do not change. In general, the coefficients of expansion of the two materials forming the compound bar will be different so that as the temp. rises each material will attempt to expand by different amounts. Figure below shows the positions to which the individual materials will expand if they are completely free to expand (i.e not joined rigidly together as a compound bar). The extension of any Length L is given by L t In general, changes in lengths due to thermal strains may be calculated form equation t = Lt, provided that the members are able to expand or contract freely, a situation that exists in statically determinates structures. As a consequence no stresses are generated in a statically determinate structure when one or more members undergo a uniform temperature change. If in a structure (or a compound bar), the free expansion or contraction is not allowed then the member becomes s statically indeterminate, which is just being discussed as an example of the compound bar and thermal stresses would be generated. Thus the difference of free expansion lengths or so called free lengths = B.L. t s .L .t = ( Bs ).L .t Since in this case the coefficient of expansion of the brass B is greater then that for the steel s. the initial lengths L of the two materials are assumed equal. If the two materials are now rigidly joined as a compound bar and subjected to the same temp. rise, each materials will attempt to expand to its free length position but each will be affected by the movement of the other. The higher coefficient of expansion material (brass) will therefore, seek to pull the steel up to its free length position and conversely, the lower coefficient of expansion martial (steel) will try to hold the brass back. In practice a compromised is reached, the compound bar extending to the position shown in fig (c), resulting in an effective compression of the brass from its free length position and an effective extension of steel from its free length position. Therefore, from the diagrams,we may conclude thefollowing Conclusion 1. Extension of steel + compression brass = difference in “ free” length Applying Newton 's law of equal action and reaction the following second Conclusion also holds good. Conclusion 2. The tensile force applied to the short member by the long member is equal in magnitude to the compressive force applied to long member by the short member.Thus in this case Tensile force in steel = compressive force in brass These conclusions may be written in the form of mathematical equations as given below: Using these two equations, the magnitude of the stresses may be determined.

Similar